OPEN Preparation of graphene nanocomposites from aqueous silver nitrate using graphene oxide’s peroxidase-like and carbocatalytic properties Kunal Garg1,5, Petri Papponen1,6, Andreas Johansson2,3,6, Nitipon Puttaraksa4 & Leona Gilbert1,5*
The present study evaluates the role of graphene oxide’s (GO’s) peroxidase-like and inherent/
GO required hydrogen peroxide (H2O2) and ammonia (NH3) in pH 4.0 disodium hydrogen phosphate (Na2HPO4). Carbocatalytic abilities of GO were triggered in pH 4.0 deionised distilled water (ddH2O). Transmission electron microscope (TEM), scanning electron microscope (SEM), cyclic voltammetry (CV) and UV-Vis spectroscopy aided in qualitatively and quantitatively assessing GO/Ag nanocomposites. TEM and SEM analysis demonstrated the successful use of GO’s peroxidase-like and carbocatalytic properties to produce GO/Ag nanocomposite. UV-Vis analysis indicated a higher yield in optical density values for GO/Ag nanocomposites created using GO’s carbocatalytic ability rather than its peroxidase- like counterpart. Additionally, CV demonstrated that GO/Ag nanocomposite fabricated here is a product of an irreversible electrochemical reaction. Our study outcomes show new opportunities for GO as a standalone catalyst in biosensing. We demonstrate a sustainable approach to obtain graphene nanocomposites exclusive of harmful chemicals or physical methods.
Remarkable optical, thermal, mechanical, and electrical properties of graphene have captivated the imaginations of scientists worldwide1–4. Graphene is an ideal composite counterpart to create fexible electronics5,6, design batteries with enhanced storage capability7, prevent steel corrosion8, and shield aircraf from heat9. Real-world graphene applications have originated across several industries like the Inov-8 running trainers that employ thermal and mechanical qualities of graphene to improve their durability10. The famous sports equipment manufacturer, HEAD applied graphene to create stronger tennis rackets with lighter weight distribution10. Te BAC-Mono formula racing car also uses graphene to boost strength and reduce the mass of its body parts by 20%11. Miniaturization of biochemical assays using graphene-based sensors for research and clinical purposes is now a reality with AGILER10012. Utilization of graphene by Inov-810, HEAD10, BAC-Mono11,12, and AGILER10012 is the tip of an iceberg considering graphene’s estimated market size of $680 million by 202013. However, the reported market size for graphene was a mere $12 million in 2013, indicating that sales in the graphene industry are predominantly raw material driven14. Graphene’s annual production has peaked at 1200 tonnes per annum compared to 4600 tonnes per year of carbon fbre or carbon nanotubes14. Reported growth in the graphene industry may seem uninspiring but demonstrates the need for technological innovations that will increase graphene consumption. A surge in
1Department of Biological and Environmental Sciences, NanoScience Center, University of Jyväskylä, Jyväskylä, Finland. 2Department of Chemistry, NanoScience Center, University of Jyväskylä, Jyväskylä, Finland. 3Department of Physics, NanoScience Center, University of Jyväskylä, Jyväskylä, Finland. 4Faculty of Science and Nanoscience & Nanotechnology, Graduate Program, King Mongkut’s University of Technology Thonburi, Bangkok, Thailand. 5Te?ted Ltd, Mattilaniemi 6-8, Jyväskylä, Finland. 6These authors contributed equally:Petri Papponen and Andreas Johansson. *email: [email protected]
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 1 www.nature.com/scientificreports/ www.nature.com/scientificreports
patent and scientifc citation trends hint graphene nanocomposites as a promising area for research and applica- tion13. Unlike graphene, the role of graphene nanocomposites extends beyond improving the existing physiolog- ical properties of a host matrix13. Catalytic properties of graphene nanocomposite help generate or store energy, reduce emission from modern automobiles, and remove pollutants from water, soil, and air13,15. Currently, research on graphene nanocompos- ites heavily relies on physically or chemically coupling graphene with metal nanoparticles for utilization in a spectrum of catalytic processes16–24. Tus, understanding graphene’s role as a standalone heterogeneous carbon catalyst (i.e., carbocatalyst25) to create nanocomposites by modifying inorganic or organic compounds is required. A simple PubMed search using the term “Graphene AND catalysis” will render over 2000 scientifc articles, and the term “Graphene AND carbocatalysis” gives about ten results. Hence, less than 1% of research articles have explored graphene’s inherent or carbocatalytic properties. Density functional theory (DFT) calculations reveal the potential use of metal-free graphene to stabilize ground state molecules through non-covalent π-π interactions26. However, pure graphene does not dissolve in organic or inorganic solvents27. Tus, researchers have functionalized the graphene surface with epoxy, hydroxyl, or carboxyl groups to obtain readily soluble graphene oxide (GO)27,28. Apart from GO’s carbocatalytic applica- tions, the use of the peroxidase-like catalytic feature of GO29 is popular among researchers developing biochem- ical assays or biosensors to transform organic compounds30. Briefy, in the presence of hydrogen peroxide, GO can replace the horseradish peroxidase enzyme to reduce 3,3′,5,5′-Tetramethylbenzidine (TMB) from colour- less to blue29. Surprisingly, GO’s peroxidase-like and carbocatalytic abilities are unexplored with the inorganic elements26. As a consequence, this study has investigated GO’s peroxidase-like and natural or carbocatalytic oxidation capabilities with inorganic compounds to show new opportunities for graphene as a standalone catalyst in bio- sensing. Specifcally, the role of GO in changing silver nitrate to silver nanoparticles (Ag) to create GO/Ag nano- composite without the use of extreme physical and chemical redox methods is explained here. Materials and Methods Materials. Highly concentrated GO dissolved in water with over 95% monolayer content was purchased from 29 Graphenea, Spain . Disodium phosphate (Na2HPO4), silver nitrate (AgNO3), hydrogen peroxide (H2O2), and 29 ammonia (NH3) were purchased from Sigma-Aldrich, Finland .
Synthesis of GO/Ag nanocomposite using GO’s peroxidase-like catalytic properties. GO surroundings were tailored to stimulate its peroxidase-like catalytic properties29 and facilitate the oxidation of aqueous AgNO3 to Ag nanoparticles. Terefore, GO/Ag nanocomposite synthesis was achieved by changing the concentration of GO in the presence of AgNO3 at a constant concentration and vice versa. Firstly, diferent GO concentrations (5 µg, 10 µg, 20 µg, 40 µg, 80 µg, and 160 µg) were independently introduced along with 100 mM H2O2, 0.1 mM AgNO3, and 40 mM NH3 to a fnal volume of 1 ml in 25 mM Na2HPO4 bufer at pH 4.0 and 37 °C. Secondly, several AgNO3 concentrations (0.4 mM, 0.8 mM, 1.6 mM, 3.2 mM, 6.4 mM, and 12.8 mM) were sepa- rately added with 100 mM H2O2, 40 µg GO, and 40 mM NH3 to a fnal volume of 1 ml in 25 mM Na2HPO4 bufer at pH 4.0 and 37 °C.
Synthesis of GO/Ag nanocomposite using GO’s intrinsic or carbocatalytic abilities. Te need for Na2HPO4, H2O2, and NH3 to create GO/Ag nanocomposite was assessed by lowering Na2HPO4 concentration (25 mM, 10 mM, 5 mM, 2.5 mM, 0.5 mM, and 0 mM) in the presence of 40 µg GO, 3.2 mM AgNO3, 100 mM H2O2, and 40 mM NH3 in total 1 ml solution. Particularly, the 0 mM Na2HPO4 (i.e., ddH2O) experiment was performed with 40 µg GO and 3.2 mM AgNO3 in the presence and absence of 100 mM H2O2 and 40 mM NH3 at pH 4.0 and 25 37 °C. Without Na2HPO4, H2O2, and NH3, GO will depend on its natural abilities to convert aqueous AgNO3 to Ag nanoparticles.
Experimental setup, characterization, and data analysis. In the case of experimental controls, all reaction components were included except AgNO3 to control for GO and vice versa. Tus, experimental controls have been referred to as GO alone or AgNO3 alone hereon. Te reaction temperature for all experiments was maintained at 37 °C using a heat block, and each component was added at 15 min intervals29. Te order in which each chemical was added to Na2HPO4 bufer was GO, H2O2, AgNO3, and NH3. Further, UV-VIS spectral analysis (Perkin Elmer Lambda 650) was performed between 300 nm to 700 nm 15 min afer adding the last element. Specimens for changing GO and AgNO3 were performed in triplicates to measure average standard deviation across all wavelengths from 300 nm to 700 nm. Following equation was applied to measure the diference in absorbance between GO/Ag nanocomposite to GO or AgNO3 alone, NanocompositeC− ontrol Nanocompositet−−ocontrol percentage = × 100 Nanocomposite (1) wherein “Nanocomposite” refers to the GO/Ag nanocomposite absorbance at 450 nm and “Control” denotes matching GO or AgNO3 alone absorbance at 450 nm. Te horseradish peroxidase (HRP) enzyme reacts with 3,3’,5,5’- tetramethylbenzidine (TMB) and is detectable at 450 nm that is extensively used for various biochemical applications31,32. As GO can mimic peroxidase-like activity29, the nanocomposite-to-control percentage meas- urements were performed at 450 nm. Equation 1 was adapted from Microsof Ofce instructions for calculating percentages using the Microsof Excel. Further, cyclic voltammetry (CV) was performed to study the molecular 33 electrochemistry between GO and AgNO3. Following previously described set-up for CV , an in-house CV was
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 2 www.nature.com/scientificreports/ www.nature.com/scientificreports
created using glassy carbon electrodes as the working and counter electrodes with an Ag/AgCl reference electrode (66-EE009) from Cypress systems. A Keithley electrometer series 2400 was utilized together with a homebuilt LabView measurement program to measure current (mA) between the working and counter electrodes, as well as diference in potential (V) between the working and reference electrodes. To avoid interference from dissolved O2, the electrolyte solution was purged with N2 gas. In all CV measurements, ±3 V was applied with a step size of 10 mV and scan rate of 38 mVs−1. Visualization studies were conducted to view the nanocomposite structures and aid in elemental analysis. Transmission electron microscopy (TEM) and scanning electron microscopy (SEM) required 5 μl of sample on Formvar/carbon coated 200 mesh copper grids. In the case of TEM, digital micrographs were acquired with Jeol JEM-1400HC (Jeol, Tokyo, Japan) that is equipped with Quemesa (Olympus Sof Imaging Systems, Münster, Germany) bottom mounted CCD-camera. Chemical characterization for GO/Ag nanocomposite was achieved with Zeiss EVO-50XVP SEM that is integrated with Bruker Quantax 400 energy dispersive spectrometer (EDS). Elemental maps from EDS were obtained using Bruker AXS detector 3001 with energy resolution <133 eV (MnKa, 1000 cps). Te counts per second values in elemental maps were normalized. Image J (https://imagej.nih. gov/ij/ version 1.51) was utilized for measuring the average size of Ag nanoparticles on GO and adding a scale bar. All figures were created using Microsoft Excel (https://products.office.com/en-in/ excel version 16.32 (19120802)), Microsof PowerPoint (https://products.ofce.com/en-in/powerpoint version 16.16.3 (181015)), QtiPlot (https://www.qtiplot.com/ version 10.9), Adobe Photoshop 2020 (https://www.adobe.com/in/products/ photoshop.html version 21.0.2), and Adobe Illustrator 2020 (https://www.adobe.com/in/products/illustrator.html version 24.0.1). Results Characterization of GO/Ag nanocomposite created using GO’s peroxidase-like catalytic prop- erties. Te reaction between increasing quantities of GO (5 µg/ml, 10 µg/ml, 20 µg/ml, 40 µg/ml, 80 µg/ml, and 160 µg/ml) with 0.1 mM AgNO3, 100 mM H2O2, and 40 mM NH3 in 25 mM Na2HPO4 is linearly proportional to the rise in absorbance values seen between 300 nm to 700 nm (Fig. 1A). Nevertheless, the nanocomposite-to-con- trol percentage (Fig. 1C) at 450 nm between GO/Ag nanocomposite to corresponding GO alone drops from 77% (5 µg GO/0.1 mM AgNO3) to 2.93% (160 µg GO/0.1 mM AgNO3). Te decline in nanocomposite-to-control per- centage is observed because varying GO concentrations in the presence of 0.1 mM AgNO3 produce spectra that are only GO dominant. However, as rising concentrations of AgNO3 (0.4 mM, 0.8 mM, 1.6 mM, 3.2 mM, 6.4 mM, and 12.8 mM) are subjected to 40 µg/ml GO, 100 mM H2O2, and 40 mM NH3 in 25 mM Na2HPO4, a four-fold increase in absorbance is noted between AgNO3 alone and their respective GO/Ag nanocomposites (Fig. 1B). Te nanocomposite-to-control percentage (Fig. 1C) at 450 nm between GO/Ag nanocomposite to matching AgNO3 alone rises from 47% (40 µg GO/0.4 mM AgNO3) to 77% (40 µg GO/12.8 mM AgNO3). Terefore, var- ying AgNO3 amounts in the presence of 40 µg/ml GO yields spectra that are GO/Ag nanocomposite dominant (Fig. 1B). Additionally, Fig. 1B reveals that 40 µg/ml GO/12.8 mM AgNO3 nanocomposite spectra is the upper limit for detection as the said GO/Ag combination saturates UV-VIS spectroscopy machine’s capability to absorb. Hence, the maximum nanocomposite-to-control percentage between GO/Ag nanocomposite to GO or AgNO3 alone can be either observed at low GO quantities (5 µg GO/0.1 mM AgNO3) or at high AgNO3 concentration (40 µg GO/12.8 mM AgNO3) as depicted in Fig. 1C. Overall, the absorbance values between 300 nm to 700 nm for all GO/Ag nanocomposites created by varying GO and AgNO3 concentrations (Fig. 1A,B) were replicable when performed in triplicates with an average standard deviation of 0.008 a.u. and 0.039 a.u., respectively (Fig. S1). Electron micrograph images of GO (160 µg/ml) or AgNO3 (12.8 mM) alone (Fig. S2) were visually compared with images of GO/Ag nanocomposites (Fig. 2). Te black dots or cloud-like deposits on GO sheets in Fig. 2 are Ag nanoparticles in comparison to the clean GO sheets in Fig. S2A. Silver nanoparticles were observed exclusively on GO sheets indicating that GO plays an imperative role in oxidizing aqueous AgNO3 and act as a substrate on which the Ag nanoparticles can nucleate (Fig. 2). Although changing GO concentrations in the presence of 0.1 mM AgNO3 produce spectra that are GO dominant (Fig. 1A), silver nanoparticles can still get deposited on GO sheets (Fig. 2A–F). Nucleation of Ag nanoparticles on GO sheet was not restricted and the resulting anisotropic nanoparticles measured larger than 500 nm (Fig. 2A–F). On increasing the amounts of AgNO3, the continuous growth of Ag nanoparticles into colloidal cloud-like particles on GO sheets was noted (Fig. 2G–L). Characterization of GO/Ag nanocomposite produced using GO’s intrinsic or carbocatalytic abilities. GO can utilize its peroxidase-like catalytic property to oxidize aqueous AgNO3 to Ag nanoparticles (Figs. 1A,B, and 2). Nonetheless, the nanocomposite-to-control percentage at 450 nm between GO/Ag nanocom- posite to GO or AgNO3 alone is limited to 77% (Fig. 1C). Growing the diference in absorbance between GO/ Ag nanocomposite and GO or AgNO3 alone at 450 nm should elevate the nanocomposite-to-control percentage (Eq. 1). To assess the reagents that produce high noise, absorbance values of 25 mM Na2HPO4, 100 mM H2O2, and 3.2 mM AgNO3 were collected at 450 nm in several combinations (Fig. S3). Individually, 25 mM Na2HPO4, 100 mM H2O2, and 3.2 mM AgNO3 did not exhibit noteworthy absorbance. In contrast, a twelve-fold increase in absorbance was observed when 3.2 mM AgNO3 was introduced to 25 mM Na2HPO4 (Fig. S3). An additional three-fold rise in absorbance was noted when 100 mM H2O2 was subjected to 3.2 mM AgNO3 in 25 mM Na2HPO4. Interaction between AgNO3 and Na2HPO4 leads to high absorbance background that is further exacerbated by the addition of H2O2 (Fig. S3). Lowering Na2HPO4 concentration (25 mM, 10 mM, 5 mM, 2.5 mM, and 0.5 mM) in the presence of 3.2 mM AgNO3, 100 mM H2O2, and 40 mM NH3 gradually decreases the background pro- duced by AgNO3 controls (Fig. 3A). Similarly, the decline in Na2HPO4 concentration in the presence of 40 µg/ml GO with 3.2 mM AgNO3, 100 mM H2O2, and 40 mM NH3 steadily reduces GO/Ag nanocomposite absorbance spectra (Fig. 3A). Te nanocomposite-to-control percentage measured at 450 nm between AgNO3 alone and matching GO/Ag nanocomposite climbs from 48% for 25 mM Na2HPO4 to 87% for 0.5 mM Na2HPO4 (Fig. 3B).
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 3 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 1. Graphene oxide (GO) utilizes its peroxidase-like catalytic property to oxidize aqueous silver nitrate (AgNO3) to silver (Ag) nanoparticles. UV-VIS spectral analysis to evaluate (A) the synthesis of GO/Ag nanocomposites at diferent GO concentrations (5 µg/ml, 10 µg/ml, 20 µg/ml, 40 µg/ml, 80 µg/ml, and 160 µg/ ml) in the presence of 0.1 mM AgNO3, 25 mM Na2HPO4, 100 mM H2O2, and 40 mM NH3, (B) the synthesis of GO/Ag nanocomposites at diferent AgNO3 concentrations (0.4 mM, 0.8 mM, 1.6 mM, 3.2 mM, 6.4 mM, and 12.8 mM) in the presence of 40 µg/ml GO, 25 mM Na2HPO4, 100 mM H2O2, and 40 mM NH3, and (C) the resulting nanocomposite-to-control percentage at 450 nanometres (nm) between GO and AgNO3 together (i.e., experiment) and GO or AgNO3 alone (i.e., control) from (A,B). All chemical reactions were carried out at 37 °C in pH 4.0 solvents. Absorbance was recorded in arbitrary units (a.u.) from 300 to 700 nm. Solid lines represent absorbance due to interaction between GO and AgNO3 together (i.e., experiment) versus dashed lines indicates absorbance of either GO or AgNO3 alone (i.e., control). Figure 1 was created using Microsof Excel (https:// products.ofce.com/en-in/excel version 16.32 (19120802)), Microsof PowerPoint (https://products.ofce.com/ en-in/powerpoint version 16.16.3 (181015)), and Adobe Photoshop 2020 (https://www.adobe.com/in/products/ photoshop.html version 21.0.2).
Interestingly, GO/Ag nanocomposite’s nanocomposite-to-control percentage grows to 97% (Fig. 3B) in the absence of Na2HPO4 and H2O2 (Fig. 3A).
Electrochemical behaviour and elemental analysis of GO/Ag nanocomposite. Te electrochem- ical measurements between GO and AgNO3 in Na2HPO4 or H2O yielded cyclic voltammograms with a large capacitive current contribution due to the working electrode having a large surface area. A redox response is most visible in the presence of Na2HPO4 with an oxidation peak at 0.15 V and a reduction peak at −0.1 V (Fig. 3C). GO and AgNO3 in H2O however displays no visible redox response and GO/Ag nanocomposite seems to be fully stable (Fig. 3D). When H2O2 and NH3 is removed, the CV response shows a broad oxidation curve that suggests a sluggish electron exchange between GO and AgNO3 (Fig. 3E). In contrast, no discernible oxidation (anodic) or reduction (cathodic) curves were observed when GO or AgNO3 alone were dissolved in H2O (Fig. S4).
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 4 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 2. Nucleation of silver (Ag) nanoparticles occurs exclusively on the graphene oxide (GO) surface. Transmission electron microscope (TEM) analysis to evaluate the synthesis of GO/Ag nanocomposites at diferent GO and AgNO3 concentrations. Various GO concentrations include (A) 5 µg/ml GO, (B) 10 µg/ml GO, (C) 20 µg/ml GO, (D) 40 µg/ml GO, (E) 80 µg/ml GO, and (F) 160 µg/ml GO in the presence of 0.1 mM AgNO3, 25 mM Na2HPO4, 100 mM H2O2, and 40 mM NH3. Similarly, several concentrations for AgNO3 include (G) 0.4 mM AgNO3, (H) 0.8 mM AgNO3, (I) 1.6 mM AgNO3, (J) 3.2 mM AgNO3, (K) 6.4 mM AgNO3, and (L) 12.8 mM AgNO3 in the presence of 40 µg/ml GO, 25 mM Na2HPO4, 100 mM H2O2, and 40 mM NH3. All chemical reactions were carried out at 37 °C in pH 4.0 solvents. Bar 500 nm. Figure 2 was compiled with the help of Image J (https://imagej.nih.gov/ij/ version 1.51) and Adobe Photoshop 2020 (https://www.adobe.com/in/ products/photoshop.html version 21.0.2).
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 5 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 3. Graphene oxide (GO)/silver (Ag) nanocomposite results from an irreversible electrochemical reaction that demonstrates the largest diference in absorbance without di-sodium hydrogen phosphate (Na2HPO4), hydrogen peroxide (H2O2), and ammonia (NH3). UV-VIS spectral analysis to evaluate (A) the synthesis of GO/Ag nanocomposites at diferent Na2HPO4 concentrations (25 mM, 10 mM, 5 mM, 2.5 mM, 0.5 mM, and 0 mM) in the presence of 40 µg/ml GO, 3.2 mM AgNO3, 100 mM H2O2, and 40 mM NH3. Specifcally, the 0 mM Na2HPO4 (i.e., H2O) experiment was performed with 40 µg/ml GO and 3.2 mM AgNO3 in the presence and absence of 100 mM H2O2, and 40 mM NH3 and has been indicated with dark red stars, and (B) the resulting nanocomposite-to-control percentage at 450 nanometres (nm) between GO and AgNO3 together (i.e., experiment) and GO or AgNO3 alone (i.e., control) from Fig. 1A,B. Further, cyclic voltammograms for 40 µg/ml GO and 3.2 mM AgNO3 with (C) 25 mM Na2HPO4, 100 mM H2O2, and 40 mM NH3, (D) H2O, 100 mM H2O2, and 40 mM NH3, and (E) H2O without 100 mM H2O2 and 40 mM NH3 indicates electrochemical irreversibility. All chemical reactions were carried out at 37 °C in pH 4.0 solvents. Absorbance was recorded in arbitrary units (a.u.) from 300 to 700 nm. Solid lines represent absorbance due to interaction between GO and AgNO3 together (i.e., experiment) versus dashed lines indicates absorbance of either GO or AgNO3 alone (i.e., control). In all CV measurements, ±3 V was applied with a step size of 10 mV and scan rate of 38 mVs−1. Image J (https://imagej.nih.gov/ij/ version 1.51) was utilized for measuring the average size of Ag nanoparticles on GO and adding a scale bar. Figure 3 was assembled using Microsof Excel (https://products.ofce.com/en-in/ excel version 16.32 (19120802)), Microsof PowerPoint (https://products.ofce.com/en-in/powerpoint version
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 6 www.nature.com/scientificreports/ www.nature.com/scientificreports
16.16.3 (181015)), QtiPlot (https://www.qtiplot.com/ version 10.9), Adobe Photoshop 2020 (https://www.adobe. com/in/products/photoshop.html version 21.0.2), and Adobe Illustrator 2020 (https://www.adobe.com/in/ products/illustrator.html version 24.0.1).
Te result of electrochemical behaviour between GO and AgNO3 can be seen in the electron micrographs pre- sented in Fig. 4. TEM images visibly indicate the deposition of silver nanoparticles on GO sheets in the absence of Na2HPO4 (Fig. 4B) and H2O2 (Fig. 4C) that is comparable to GO/Ag nanocomposite created in 25 mM Na2HPO4 (Figs. 2 and 4A). Additionally, the presence of silver nanoparticles on GO sheets was confrmed with SEM and EDS (Fig. 5). Here the GO/Ag nanocomposite appears bright compared to the darker background of formvar. Mapping of elements was performed either on (black star) or around (grey star) the GO/Ag nanocomposite (Fig. 5A–C). Similarly, elemental maps include a black or grey line to correspond with said coloured EDS meas- urement stars (Fig. 5A.1–C.1). Elemental mapping on GO/Ag nanocomposite (black star and line) consistently demonstrated peaks for Carbon (C at 0.28 keV), Oxygen (O at 0.53 keV), Copper (Cu at 0.93 keV), Aluminium (Al at 1.49 keV), and Silver (Ag at 2.99 keV, 3.17 keV, and 3.33 keV). Te EDS measurements around GO/Ag nano- composite (grey star and line) did not yield any Cu or Ag peaks, while the C and O peaks are consistent with the underlying formvar. Figure 5D,D.1 indicate that GO is the source for Cu, as also seen in GO/Ag nanocomposite elemental maps (Fig. 5A.1–C.1). Further, Al was seen in all EDS measurements due to the sample holder beneath the formvar copper grid. Figure 6 illustrates a comparison between the synergistic and inherent catalytic approaches for creating graphene nanocomposites. Furthermore, Fig. 7 proposes a mechanism to understand the surface chemistry involved in oxidizing AgNO3 to Ag nanoparticles. Discussion We demonstrate the use of GO’s peroxidase-like29 and inherent or carbocatalytic properties25 to oxidize inor- ganic compounds such as AgNO3. Te Na2HPO4 bufer with H2O2 activates the peroxidase-like catalytic property of GO that converts AgNO3 to Ag nanoparticles (Figs. 1 and 2). Te nanocomposite-to-control percentage for resulting GO/Ag nanocomposite is a maximum of 77% (Fig. 1C) because the interaction between Na2HPO4 and AgNO3 produces high noise (Fig. S3). In contrast, GO/Ag nanocomposite created in deionized distilled water (pH 4.0) without H2O2 yields 97% in nanocomposite-to-control diference (Fig. 3B). In the absence of Na2HPO4 and H2O2, GO’s intrinsic ability facilitates the transformation of AgNO3 to Ag nanoparticles (Figs. 3–5). Large aromatic basal planes of GO ofer a high surface area containing epoxy, hydroxyl, and carboxyl functional groups 25 that contribute to GO’s inbuilt catalytic properties . Our fndings indicate that GO alone can oxidize AgNO3 and also act as a substrate for Ag nanoparticles to generate GO/Ag nanocomposites. Te GO/Ag nanocomposite created in this study using only natural catalytic properties of GO is simple, resource-efcient, and swif compared to old techniques (Fig. 6). Traditionally, synthesis of GO nanocompos- ites with metal nanoparticles as shown in Fig. 6 includes pre-treatment of GO, organic/inorganic solvents to dissolve the metal precursor, and chemical/physical methods to reduce and stabilize the fnal product16–24. GO pre-treatment may involve adsorption or electrodeposition of metal ions16, conjugation with antibodies17, PEG19, 18,23 16 21 and more . Further, solvents of metal precursors such as AgNO3 , chloroplatinic acid (H2PTCL6) , and cobalt 22 19 22 17 16 (II) acetate (Co(CH3COO)2) include deionized distilled water , ethanol , 1% BSA , citrate bufer , or sul- phuric acid23. Ultimately, blending of GO with metal nanoparticles demands the presence of chemical agents like 16,17 20 24 22 hydroquinone , hydrazine hydrate , sodium borohydride (NaBH4) , or ammonium hydroxide (NH4OH) to reduce and stabilize the metal clusters on GO surface. Alternatively, extreme physical methods such as auto- clave15,22, annealing or heating at 60 °C to 600 °C19,20,23 have been reported to create metal nanoparticles over GO. Catalytic properties of GO are either synergistic or inherent following the literature15 and our research fnd- ings (Figs. 4–6). A synergistic approach advocates the integration of GO with other catalytic components such as silver16, palladium20, platinum21, or cobalt22 nanoparticles using pre-treated GO16–20,23, chemical agents16,17,20–22,24, or heating19,20,22,23. As a result, GO in synergy with metal nanoparticles participates in photocatalysis24, pho- todegradation23, bactericidal activity16, Suzuki-Miyaura coupling reaction20, oxygen evolution reaction22, and 21 22 methanol or oxygen oxidation reaction . In contrast, the oxidation of AgNO3 to Ag nanoparticles in this study is infuenced by the functional group composition, structure, and morphology of GO (Figs. 3–5) that signifes its inherent catalytic properties25. Application of GO’s intrinsic catalytic abilities is limited to either hydration or oxidation of various organic compounds, including alcohols, alkynes, and alkenes34. Additionally, the use of heteroatom doped GO in oxygen reduction reactions is considered as a natural use of GO’s catalytic abilities34–36. However, attaching heteroatoms like sulphur36 and iodine35 to GO also comprises several pre-treatment processes as vigorous ultrasonication, and annealing at 500 °C to 1100 °C in an argon atmosphere35,36. Te GO/Ag nanocomposite fabricated here is a product of an electrochemical irreversible reaction (Fig. 3C,D). Kinetics that may govern the irreversible nucleation, growth, and attachment of Ag nanoparticles on GO (Fig. 7) can be described in three steps (1) monomer supplying reaction, (2) growth by difusion and (3) autocatalytic oxi- dation37,38. Same three steps also explain the development of gold nanoparticles in a classical Turkevich method wherein citrate and squaric or ascorbic acid are used as reducing agents37–43. Te monomer supplying reaction 37,38 (Fig. 7) is imperative for making Ag monomers/ions and clusters . Primary contact between AgNO3 and func- tional groups of GO may initiate the creation of many Ag monomers over GO. Coalescence follows the creation of Ag monomers due to the low aggregation barrier to form frst clusters or Ag seed particles (Fig. 7). Lower or higher aggregation barrier is essentially activation energy that either promotes coalescence among monomers or inhibits aggregation between large nanoparticles, respectively37,38,40. In the next step, newly formed Ag mono- mers may difuse onto the existing seed particles to facilitate the growth phase of Ag nanoparticles over GO38,40.
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 7 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 4. Graphene oxide (GO) utilizes its intrinsic or carbocatalytic ability to oxidize aqueous silver nitrate (AgNO3) to silver (Ag) nanoparticles in the absence of di-sodium hydrogen phosphate (Na2HPO4), hydrogen peroxide (H2O2), and ammonia (NH3). Transmission electron microscope (TEM) analysis to evaluate the facile synthesis of GO/Ag nanocomposites in (A) 25 mM Na2HPO4 with 100 mM H2O2 and 40 mM NH3, (B) H2O with 100 mM H2O2 and 40 mM NH3, (C) H2O without 100 mM H2O2 and 40 mM NH3. All chemical reactions were carried out at 37 °C in pH 4.0 solvents using 40 µg/ml GO with 3.2 mM AgNO3. Bar 500 nm. Figure 4 was compiled with the help of Image J (https://imagej.nih.gov/ij/ version 1.51) and Adobe Photoshop 2020 (https:// www.adobe.com/in/products/photoshop.html version 21.0.2).
Difusion rate for the growth of Ag nanoparticles may strongly depend on the amount of Ag monomers that are supplied to standing clusters (Fig. 7). Lastly, autocatalytic oxidation comprises the constant reiteration of steps 37,38 one and two till remaining AgNO3 is consumed to obtain the fnal Ag nanoparticles .
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 8 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 5. Scanning electron microscopy (SEM) and energy dispersive spectrometer (EDS) provide empirical evidence for graphene oxide (GO)/silver (Ag) nanocomposite fabrication. SEM micrographs indicates the synthesis of GO/Ag nanocomposites in (A) 25 mM Na2HPO4 with 100 mM H2O2 and 40 mM NH3, (B) H2O with 100 mM H2O2 and 40 mM NH3, (C) H2O without 100 mM H2O2 and 40 mM NH3, and (D) GO alone. Te black and grey stars in Fig. 5A–D indicate the place for EDS measurements that directly corresponds with the black and dashed grey lines in elemental maps for GO/Ag nanocomposites in (A.1) 25 mM Na2HPO4 with 100 mM H2O2 and 40 mM NH3, (B.1) H2O with 100 mM H2O2 and 40 mM NH3, (C.1) H2O without 100 mM H2O2 and 40 mM NH3, and (D.1) GO alone. All chemical reactions were carried out at 37 °C in pH 4.0 solvents using 40 µg/ml GO with 3.2 mM AgNO3. Bar 500 nm. Figure 5 was created using Microsof PowerPoint (https:// products.ofce.com/en-in/powerpoint version 16.16.3 (181015)), Adobe Photoshop 2020 (https://www.adobe. com/in/products/photoshop.html version 21.0.2), and Adobe Illustrator 2020 (https://www.adobe.com/in/ products/illustrator.html version 24.0.1).
Unlike the Turkevich method37–42, the size, shape, density, and distribution of Ag nanoparticles on GO is not homogenous in our study. Nonetheless, heterogenous GO/Ag nanocomposites have produced replicable results when characterized using UV-VIS spectroscopy (Fig. S1). Te growth by difusion step is crucial for narrowing polydispersity among gold nanoparticles that are produced in suspension using the Turkevich method37–42. In
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 9 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 6. Graphene oxide (GO)/metal nanocomposites can be achieved without the use of harmful chemicals and extreme physical reduction methods. Schematic comparing key requirements to generate GO/metal nanocomposites following reported methodologies (old approach) versus current technique (new approach). Figure 6 was created using Microsof PowerPoint (https://products.ofce.com/en-in/powerpoint version 16.16.3 (181015)), Adobe Photoshop 2020 (https://www.adobe.com/in/products/photoshop.html version 21.0.2), and Adobe Illustrator 2020 (https://www.adobe.com/in/products/illustrator.html version 24.0.1).
contrast, nucleation and growth of Ag nanoparticles are restricted by GO’s fnite sheet size (Figs. 2, S2, 5) and island-like arbitrary distribution44,45 of active sites (i.e., epoxy, hydroxyl, and carboxyl functional groups). Also, the size and density of Ag nanoparticles on GO is determined by the starting quantity of AgNO3 (Fig. 7). Small amounts of raw AgNO3 are readily converted to Ag nanoparticles that are distinguishable (Fig. 7A). However,
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 10 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 7. Silver (Ag) nanoparticle growth on graphene oxide (GO) is due to coalescence. Schematic illustration of surface chemistry and the mechanism postulated to be involved in GO/Ag nanocomposite synthesis due to coalescence with (A) small, and (B) large amounts of AgNO3. Figure 7 was created using Microsof PowerPoint (https://products.ofce.com/en-in/powerpoint version 16.16.3 (181015)), Adobe Photoshop 2020 (https://www. adobe.com/in/products/photoshop.html version 21.0.2), and Adobe Illustrator 2020 (https://www.adobe.com/ in/products/illustrator.html version 24.0.1).
larger quantities of AgNO3 are transformed to Ag cloud-like nanoparticles that prominently cover the GO sheets (Fig. 7B). Cloud-like nanoparticles may result due to sizeable AgNO3 residual that is continuously oxidized to Ag monomers and difused onto the existing Ag nanoparticles (i.e., autocatalytic oxidation) over a fnite size of GO sheet (Fig. 7B). Among various inorganic compounds, applications of silver nanoparticles in the biomedical feld is wide- spread and ever-increasing due to its low-cost, abundance, and fascinating properties46,47. As a consequence, silver nitrate was utilized in this study to embody GO’s peroxidase-like and natural or carbocatalytic oxidation capabilities with inorganic compounds. However, as Ag is monovalent, more research is required to understand the limits of GO’s peroxidase-like or intrinsic catalytic properties using divalent, trivalent, and tetravalent inor- ganic elements48. Te intrinsic and peroxidase-like catalytic properties of graphene shown here may be seen in its allotropes like carbon nanotubes49–52 and fullerenes53 coupled with epoxy, hydroxyl, and carboxyl groups. Also, in future experiments, radical scavenger study and electron spin resonance technique can help understand the infuence of free radicals, O2, and OH groups (i.e., resulting from decomposed H2O2) on the fabrication of carbon nanocomposites. What plastic was for the 20th century, graphene is to the 21st century. Te World Bank and the United Nations have adopted several sustainable development goals to reduce the risk that plastic poses to our environment and public health54. Currently, the lack of standardized health and safety guidelines to assess the toxic infuence of unique graphene-based technologies on human health and the environment is staggering14. In Europe, the registration, evaluation, authorization, and restriction of chemicals (REACH) regulation (EC 1907/2006) by the European Agency for Safety and Health at Work instructs wellbeing at organizations that manufacture or import harmful chemicals55. Nonetheless, the REACH regulation only applies to establishments dealing with one tonne or more graphene per year14. In 2017, the International Organization for Standards (ISO) published ISO/TS 80004:13:201756 that only clarifes technical pre-requisites for a material to be deemed as graphene or otherwise.
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 11 www.nature.com/scientificreports/ www.nature.com/scientificreports
Given the inevitable mass application of graphene and missing guidelines to prevent public health hazards and environmental risks, the research community may become the frontline in consciously assessing the carbon footprint of their innovations. In the spirit of new opportunities for graphene in catalysis like biosensing, we show that using GO’s standalone catalytic abilities will reduce the widespread dependence on harmful chemicals and extreme physical methods to obtain graphene nanocomposites. Data availability All available data in present article has been illustrated through Figs. 1 to 7 and Figures S1 to S4.
Received: 28 October 2019; Accepted: 25 February 2020; Published: xx xx xxxx
References 1. Ghuge, A. D., Shirode, A. R. & Kadam, V. J. Graphene: A Comprehensive Review. Curr. Drug. Targets. 18, 724–733 (2017). 2. Ahmadivand, A., Gerislioglu, B. & Ramezani, Z. Gated graphene island-enabled tunable charge transfer plasmon terahertz metamodulator. Nanoscale. 11, 8091–8095 (2019). 3. Wu, T., Luo, Y., Maier, S. A. & Wei, L. Phase-matching and Peak Nonlinearity Enhanced Tird-Harmonic Generation in Graphene Plasmonic Coupler. Phys. Rev. Appl. 11, 014049 (2019). 4. Ahmadivand, A., Gerislioglu, B., Noe, T. G. & Mishra, Y. Gated Graphene Enabled Tunable Charge–Current Confgurations in Hybrid Plasmonic Metamaterials. Acs Appl. Electron. Mater. 1, 637–641 (2019). 5. Ahn, J.-H. & Hong, B. Graphene for displays that bend. Nat. Nanotechnol. 9, 737–738 (2014). 6. Polat, E. O. et al. Flexible graphene photodetectors for wearable ftness monitoring. Sci. Adv. 5, eaaw7846 (2019). 7. Liu, J. Charging graphene for energy. Nat. Nanotechnol. 9, 739–741 (2014). 8. Böhm, S. Graphene against corrosion. Nat Nanotechnol. 9, nnano.2014.220 (2014). 9. Siochi, E. J. Graphene in the sky and beyond. Nat Nanotechnol. 9, nnano.2014.231 (2014). 10. Kronsberg, M. Hyped miracle material graphene is realizing its promise as ‘Pixie Dust’. (2018). 11. Kew, O. You can’t have the new, lighter, faster BAC Mono R. (2019). 12. Goldsmith, B. R. et al. Digital Biosensing by Foundry-Fabricated Graphene Sensors. Sci. Rep-uk. 9, 434 (2019). 13. Dhand, V., Rhee, K., Kim, H. & Jung, D. A Comprehensive Review of Graphene Nanocomposites: Research Status and Trends. J. Nanomater. 2013, 1–14 (2013). 14. Zurutuza, A. & Marinelli, C. Challenges and opportunities in graphene commercialization. Nat. Nanotechnol. 9, 730–734 (2014). 15. Huang, C., Li, C. & Shi, G. Graphene based catalysts. Energ. Env. Sci. 5, 8848–8868 (2012). 16. Bao, Q., Zhang, D. & Qi, P. Synthesis and characterization of silver nanoparticle and graphene oxide nanosheet composites as a bactericidal agent for water disinfection. J. Colloid Interf. Sci. 360, 463–470 (2011). 17. Wan, Y., Wang, Y., Wu, J. & Zhang, D. Graphene Oxide Sheet-Mediated Silver Enhancement for Application to Electrochemical Biosensors. Anal. Chem. 83, 648–653 (2011). 18. Yagati, A. et al. Silver nanofower–reduced graphene oxide composite based micro-disk electrode for insulin detection in serum. Biosens. Bioelectron. 80, 307–314 (2016). 19. Rong, X. et al. A nanocomposite, a fltration membrane comprising the nanocomposite, and methods to form the nanocomposite and the fltration membrane. World Intellectual Property Organization. WO2012177223A1 (2012). 20. Scheuermann, G. M., Rumi, L., Steurer, P., Bannwarth, W. & Mulhaupt, R. Palladium Nanoparticles on Graphite Oxide and Its Functionalized Graphene Derivatives as Highly Active Catalysts for the Suzuki−Miyaura Coupling Reaction. J. Am. Chem. Soc. 131, 8262–8270 (2009). 21. Li, Y., Tang, L. & Li, J. Preparation and electrochemical performance for methanol oxidation of pt/graphene nanocomposites. Electrochem. Commun. 11, 846–849 (2009). 22. Liang, Y. et al. Co3O4 nanocrystals on graphene as a synergistic catalyst for oxygen reduction reaction. Nat. Mater. 10, 780 (2011). 23. Li, N. et al. Battery Performance and Photocatalytic Activity of Mesoporous Anatase TiO2 Nanospheres/Graphene Composites by Template-Free Self-Assembly. Adv. Funct. Mater. 21, 1717–1722 (2011). 24. Mukherji, A., Seger, B., Lu, G. & Wang, L. Nitrogen Doped Sr2Ta2O7Coupled with Graphene Sheets as Photocatalysts for Increased Photocatalytic Hydrogen Production. Acs Nano. 5, 3483–3492 (2011). 25. Navalon, S., Dhakshinamoorthy, A., Alvaro, M. & Garcia, H. Carbocatalysis by Graphene-Based Materials. Chem. Rev. 114, 6179–6212 (2014). 26. Kroeger, A. A. & Karton, A. Catalysis by pure graphene – From supporting actor to protagonist through shape complementarity. J Org Chem. (2019). 27. Neklyudov, V. V., Khafzov, N. R., Sedov, I. A. & Dimiev, A. M. New insights into the solubility of graphene oxide in water and alcohols. Phys. Chem Chem Phys. 19, 17000–17008 (2017). 28. Zaaba, N. I. et al. Synthesis of Graphene Oxide using Modifed Hummers Method: Solvent Infuence. Procedia. Engineer. 184, 469–477 (2017). 29. Song, Y., Qu, K., Zhao, C., Ren, J. & Qu, X. Graphene Oxide: Intrinsic Peroxidase Catalytic Activity and Its Application to Glucose Detection. Adv. Mater. 22, 2206–2210 (2010). 30. Garg, B., Bisht, T. & Ling, Y.-C. Graphene-Based Nanomaterials as Efficient Peroxidase Mimetic Catalysts for Biosensing Applications: An Overview. Molecules. 20, 14155–14190 (2015). 31. Andreasson, U. et al. A Practical Guide to Immunoassay Method Validation. Front. Neurol. 6, 179 (2015). 32. Crowther, J. R. Te ELISA Guidebook. Humana Press Inc. 149, 415 (Humana Press Inc., 2001). 33. Elgrishi, N. et al. A Practical Beginner’s Guide to Cyclic Voltammetry. J Chem Educ. https://doi.org/10.1021/acs.jchemed.7b00361 (2017). 34. Dreyer, D. R., Jia, H. & Bielawski, C. W. Graphene Oxide: A Convenient Carbocatalyst for Facilitating Oxidation and Hydration Reactions. Angew. Chem. Int. Ed. 49, 6813–6816 (2010). 35. Yao, Z. et al. Catalyst -free synthesis of iodine-doped graphene via a facile thermal annealing process and its use for electrocatalytic oxygen reduction in an alkaline medium. Chem. Commun. 48, 1027–1029 (2011). 36. Yang, Z. et al. Sulfur-Doped Graphene as an Efcient Metal-free Cathode Catalyst for Oxygen Reduction. Acs Nano. 6, 205–211 (2012). 37. Polte, J. et al. Mechanism of Gold Nanoparticle Formation in the Classical Citrate Synthesis Method Derived from Coupled In Situ XANES and SAXS Evaluation. J. Am. Chem. Soc. 132, 1296–1301 (2010). 38. Polte, J. Fundamental growth principles of colloidal metal nanoparticles – a new perspective. Crystengcomm. 17, 6809–6830 (2015). 39. Turkevich, J., Stevenson, P. & Hillier, J. A study of the nucleation and growth processes in the synthesis of colloidal gold. Discuss. Faraday Soc. 11, 55–75 (1951). 40. Kumar, S., Gandhi, K. & Kumar, R. Modeling of Formation of Gold Nanoparticles by Citrate Method. Ind. Eng. Chem. Res. 46, 3128–3136 (2007).
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 12 www.nature.com/scientificreports/ www.nature.com/scientificreports
41. Pong, B.-K. et al. New Insights on the Nanoparticle Growth Mechanism in the Citrate Reduction of Gold(III) Salt: Formation of the Au Nanowire Intermediate and Its Nonlinear Optical Properties. J. Phys. Chem. C. 111, 6281–6287 (2007). 42. Mikhlin, Y. et al. Submicrometer intermediates in the citrate synthesis of gold nanoparticles: New insights into the nucleation and crystal growth mechanisms. J. Colloid Interf. Sci. 362, 330–336 (2011). 43. Larm, N. E. et al. Room-Temperature Turkevich Method: Formation of Gold Nanoparticles at the Speed of Mixing Using Cyclic Oxocarbon Reducing Agents. J. Phys. Chem. C. 122, 5105–5118 (2018). 44. Shin, D. et al. Distribution of oxygen functional groups of graphene oxide obtained from low-temperature atomic layer deposition of titanium oxide. Rsc Adv. 7, 13979–13984 (2017). 45. Tararan, A., Zobelli, A., Benito, A. M., Maser, W. K. & Stéphan, O. Revisiting Graphene Oxide Chemistry via Spatially-Resolved Electron Energy Loss Spectroscopy. Chem. Mater. 28, 3741–3748 (2016). 46. Lee, S. & Jun, B.-H. Silver Nanoparticles: Synthesis and Application for Nanomedicine. Int. J. Mol. Sci. 20, 865 (2019). 47. Burdușel, A.-C. et al. Biomedical Applications of Silver Nanoparticles: An Up-to-Date Overview. J. Nanomater. 8, 681 (2018). 48. Liu, X. et al. Metals on Graphene: Interactions, Growth Morphology, and Termal Stability. Crystals. 3, 79–111 (2013). 49. Liu, Z. et al. Carboxylation of multiwalled carbon nanotube enhanced its biocompatibility with L02 cells through decreased activation of mitochondrial apoptotic pathway. J. Biomed. Mater. Res. A. 102, 665–673 (2014). 50. Das, G. et al. Fluorescent microspheres of zinc 1,2-dicarbomethoxy-1,2-dithiolate complex decorated with carbon nanotubes. Carbon Lett. 29, 595–603 (2019). 51. Begum, A., Tripathi, K. M. & Sarkar, S. Water-Induced Formation, Characterization, and Photoluminescence of Carbon Nanotube- Based Composites of Gadolinium(III) and Platinum(II) Dithiolenes. Chem. - Eur. J. 20, 16657–16661 (2014). 52. Tripathi, K., Begum, A., Sonkar, S. & Sarkar, S. Nanospheres of copper(iii) 1,2-dicarbomethoxy-1,2-dithiolate and its composite with water soluble carbon nanotubes. N. J. Chem. 37, 2708 (2013). 53. Semenov, K. N. et al. Carboxylated fullerenes: Physico-chemical properties and potential applications. Prog. Solid. State Ch. 47, 19–36 (2017). 54. Westerbos, M. How the Sustainable Development Goals Can Help Fight ‘Plastic Soup’. (2019). 55. EU Commission. Te registration, evaluation, authorization, and restriction of chemicals regulation (REACH). (2006). 56. ISO. ISO/TS 80004–13:2017 Nanotechnologies – Vocabulary – Part 13: Graphene and Related Two-Dimensional (2D) Materials. 21 (2017). Acknowledgements Tis study was supported by the Schwartz Foundation and the Finnish Innovation Funding Agency TEKES TUTL project number 774/31/2015. Te funders had no role in study design, data collection, and analysis, decision to publish, or preparation of the manuscript. We acknowledge that the reviewer’s comments have helped improve the overall quality of our article. Lastly, we thank Jyrki Manninen from the Physics department at the University of Jyväskylä for his help with the cyclic voltammetry measurements. Author contributions K.G., P.P., A.J., N.P. and L.G. contributed to the design and analysis of experiments. K.G., P.P., A.J. and L.G. performed the experiments in this manuscript. K.G., A.J. and L.G. wrote the manuscript. K.G., P.P., A.J., N.P. and L.G. critically reviewed the manuscript. Competing interests Yes, the authors have competing interests as defned by the Scientifc Reports Journal, or other interests that might be perceived to infuence the results and/or discussion reported in this paper. Following Scientifc Reports policy authors of this manuscript have the following competing interests, KG and LG have a fnancial and business interest in Te?ted Oy. PP, AJ, and NP have no commercial or fnancial relationships that could be construed as a potential confict of interest. Funding sources mentioned in the acknowledgment section and Te?ted Oy had no role in experimental design, reporting of the results, or the decision to publish. Additional information Supplementary information is available for this paper at https://doi.org/10.1038/s41598-020-61929-9. Correspondence and requests for materials should be addressed to L.G. Reprints and permissions information is available at www.nature.com/reprints. Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afliations. Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Cre- ative Commons license, and indicate if changes were made. Te images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not per- mitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
© Te Author(s) 2020
Scientific Reports | (2020) 10:5126 | https://doi.org/10.1038/s41598-020-61929-9 13